- Laser beam welding
Laser beam welding (LBW) is a
weldingtechnique used to join multiple pieces of metal through the use of a laser. The beam provides a concentrated heat source, allowing for narrow, deep welds and high welding rates. The process is frequently used in high volume applications, such as in the automotive industry.
electron beam welding(EBW), laser beam welding has high power density (on the order of 1 Megawatt/cm²(MW)) resulting in small heat-affected zones and high heating and cooling rates. The spot size of the laser can vary between 0.2 mm and 13 mm, though only smaller sizes are used for welding. The depth of penetration is proportional to the amount of power supplied, but is also dependent on the location of the focal point: penetration is maximized when the focal point is slightly below the surface of the workpiece.
A continuous or pulsed laser beam may be used depending upon the application. Milliseconds long pulses are used to weld thin materials such as razor blades while continuous laser systems are employed for deep welds.
LBW is a versatile process, capable of welding
carbon steels, HSLA steels, stainless steel, aluminum, and titanium. Due to high cooling rates, cracking is a concern when welding high-carbon steels. The weld quality is high, similar to that of electron beam welding. The speed of welding is proportional to the amount of power supplied but also depends on the type and thickness of the workpieces. The high power capability of gas lasers make them especially suitable for high volume applications. LBW is particularly dominant in the automotive industry. [Cary and Helzer, p 210] [Weman, p 97]
Some of the advantages of LBW in comparison to EBW are as follows: the laser beam can be transmitted through air rather than requiring a vacuum, the process is easily automated with robotic machinery, x-rays are not generated, and LBW result in higher quality welds.
A derivative of LBW,
laser-hybrid welding, combines the laser of LBW with an arc welding method such as gas metal arc welding. This combination allows for greater positioning flexibility, since GMAW supplies molten metal to fill the joint, and due to the use of a laser, increases the welding speed over what is normally possible with GMAW. Weld quality tends to be higher as well, since the potential for undercutting is reduced. [Weman, p 98]
*The two types of lasers commonly used in are
solid-state lasers and gas lasers (especially carbon dioxide lasers and lasers).
*The first type uses one of several solid media, including synthetic ruby and
chromiumin aluminum oxide, neodymiumin glass (Nd:glass), and the most common type, crystal composed of yttrium aluminum garnetdoped with neodymium (Nd:YAG).
*Gas lasers use mixtures of gases like
helium, nitrogen, and carbon dioxide(CO2 laser) as a medium.
*Regardless of type, however, when the medium is excited, it emits photons and forms the laser beam.
olid state laser
Solid-state lasers operate at wavelengths on the order of 1 micrometer, much shorter than gas lasers, and as a result require that operators wear special eyewear or use special screens to prevent
retinadamage. Nd:YAG lasers can operate in both pulsed and continuous mode, but the other types are limited to pulsed mode. The original and still popular solid-state design is a single crystal shaped as a rod approximately 20 mm in diameter and 200 mm long, and the ends are ground flat. This rod is surrounded by a flash tubecontaining xenonor krypton. When flashed, a pulse of light lasting about two milliseconds is emitted by the laser. Disk shaped crystals are growing in popularity in the industry, and flashlamps are giving way to diodes due to their high efficiency. Typical power output for ruby lasers is 10–20 W, while the Nd:YAG laser outputs between 0.04–6,000 W. To deliver the laser beam to the weld area, fiber optics are usually employed.
Gas lasers use high-voltage, low-current power sources to supply the energy needed to excite the gas mixture used as a lasing medium. These lasers can operate in both continuous and pulsed mode, and the wavelength of the laser beam is 10.6 μm. Fiber optic cable absorbs and is destroyed by this wavelength, so a rigid lens and mirror delivery system is used. Power outputs for gas lasers can be much higher than solid-state lasers, reaching 25
kW. [Cary and Helzer, p 209]
*Cary, Howard B. and Scott C. Helzer (2005). "Modern Welding Technology". Upper Saddle River,
New Jersey: Pearson Education. ISBN 0-13-113029-3.
*Weman, Klas (2003). "Welding processes handbook". New York: CRC Press LLC. ISBN 0-8493-1773-8.
*Kalpakjian, Serope and Schmid,Steven R.(2006). "Manufacturing Engineering and Technology"5th ed. Upper Saddle River,
New Jersey: Pearson Education. ISBN 0-13-148965-8
* [http://files.aws.org/wj/supplement/10-2002-XIE-s.pdf Dual beam laser welding; research article from the 2002 Welding Journal]
* [http://files.aws.org/wj/supplement/11-2002-XIE-s.pdf Weld morphology and thermal modeling in dual-beam laser welding; research article from the 2002 Welding Journal]
* [http://www.industrial-lasers.com/laser-welding/index.html Laser welding articles from the Industrial Laser Solutions Magazine]
* [http://www.fraunhofer.de/fhg/Images/magazine1-2005-36f_tcm6-14041.pdf Laser-beam welding makes aircraft lighter;]
Fraunhofer Society[http://www.iws.fraunhofer.de/e_welcome.html Material and Beam Technology - IWS] , Dresden, Germany( 1 January 2005)
* [http://www.twi.co.uk/content/laser_welding.html Laser welding of thick sections, aluminium, plastics etc.]
Wikimedia Foundation. 2010.
Look at other dictionaries:
Laser beam welding — Laser beam welding. См. Сварка лазерным лучом. (Источник: «Металлы и сплавы. Справочник.» Под редакцией Ю.П. Солнцева; НПО Профессионал , НПО Мир и семья ; Санкт Петербург, 2003 г.) … Словарь металлургических терминов
Laser-hybrid welding — is a type of welding process that combines the principles of laser beam welding and arc welding. Introduction The combination of laser light and an electrical arc into an amalgamated welding process has beenknown since the 1970 s, but has only… … Wikipedia
Electron beam welding — (EBW) is a fusion welding process in which a beam of high velocity electrons is applied to the materials being joined. The workpieces melt as the kinetic energy of the electrons is transformed into heat upon impact, and the filler metal, if used … Wikipedia
Welding — is a fabrication process that joins materials, usually metals or thermoplastics, by causing coalescence. This is often done by melting the workpieces and adding a filler material to form a pool of molten material (the weld puddle ) that cools to… … Wikipedia
Laser cutting — process on a sheet of steel. CAD (top) and stainless steel laser cut part (bottom) Laser cutting is a technology that uses a laser to cut materials, an … Wikipedia
Laser — For other uses, see Laser (disambiguation). United States Air Force laser experiment … Wikipedia
welding — Technique for joining metallic parts, usually through the application of heat. Discovered in the 1st millennium AD during attempts to manipulate iron into useful shapes, the technique produced a strong, tough blade. Welding traditionally involved … Universalium
laser — /lay zeuhr/, n. Physics. a device that produces a nearly parallel, nearly monochromatic, and coherent beam of light by exciting atoms to a higher energy level and causing them to radiate their energy in phase. Also called optical maser. [1955 60; … Universalium
Laser applications — There are many scientific, military, medical and commercial laser applications which have been developed since the invention of the laser in the 1958. The coherency, high monochromaticity, and ability to reach extremely high powers are all… … Wikipedia
Laser diode — Top: a packaged laser diode shown with a penny for scale. Bottom: the laser diode chip is removed from the above package and placed on the eye of a needle for scale … Wikipedia